Enhanced giant magnetoimpedance in heterogeneous nanobrush
© Zhang et al.; licensee Springer. 2012
Received: 12 July 2012
Accepted: 25 August 2012
Published: 10 September 2012
A highly sensitive and large working range giant magnetoimpedance (GMI) effect is found in the novel nanostructure: nanobrush. The nanostructure is composed of a soft magnetic nanofilm and a nanowire array, respectively fabricated by RF magnetron sputtering and electrochemical deposition. The optimal GMI ratio of nanobrush is promoted to more than 250%, higher than the pure FeNi film and some sandwich structures at low frequency. The design of this structure is based on the vortex distribution of magnetic moments in thin film, and it can be induced by the exchange coupling effect between the interfaces of nanobrush.
Keywordsnanobrush giant magnetoimpedance micromagnetic simulation FMR
Giant magnetoimpedance (GMI) effect has been considered as a potential physical effect that may take the place of giant magnetoresistance (GMR) because of its higher field sensitivity and better signal intensity . Since GMI changes as the function of external dc (direct current) magnetic field or applied dc/ac (alternating current) currents, it is possible to design GMI-based sensors that can measure either magnetic fields or dc/ac currents [2, 3]. Based on the applied stress dependence of the GMI effect, new kinds of stress sensors have been proposed [4–6]. Many industrial and engineering applications of GMI sensors have been proposed and realized to date, including traffic controls, automobile uses, biomedical sensors, and so forth [7–9]. Typical materials which may give rise to GMI effect are amorphous wires, amorphous ribbon, multilayer films, and other soft magnetic materials [10–15]. Normally, the diameter of amorphous wires and the thickness of ribbons are up to micrometer scale, and the multilayer films with a high-GMI ratio work in gigahertz. In recent years, with the rapid development of nanomaterials, the size of magnetic sensors is projected to reach nanoscale. However, traditional GMI materials do not satisfy the desired size, and it is a challenge to find new kinds of nanomaterials, which can have both an obvious GMI effect and a rapid magnetic response at a low frequency.
GMI effect is normally attributed to a combination of skin effect and high sensitivity of transverse permeability to the external dc field [16, 17]. In a magnetic medium, the skin depth is dependent on the transverse magnetic permeability (μt) through , where σ and μt are the electrical conductivity and the transverse permeability of the ferromagnetic material, respectively. For amorphous ribbons and wires, many approaches have been tried to improve the GMI ratio, such as annealing, ion irradiation, glass coating, and patterning [18–20]. Essentially, all the above approaches to enhance GMI ratio are based on the changes of magnetic domain and induced transverse distribution of magnetic moments . For the films, the sandwich structure is the traditional approach to depress the skin effect and improve the GMI ratio, but the low GMI ratio and high working frequency constitute major negative factors for applications. Obviously, it is urgent to solve the problem of how to induce the transverse moment distribution and enhanced GMI ratio in the nanomaterial.
As a typical nanostructure, nanobrush, has been studied as one of the nanodevices for its special characters [21–23]. However, it is rare as far as the magnetic sensor applications are concerned. In this paper, a kind of magnetic nanobrush, consisted of nanofilm and nanowire array, is prepared. Considering that the origin of GMI is the change of transverse permeability under an external applied field, the design of the structure is based on the different vortex distributions of magnetic moments in thin film, which could be induced by the exchange coupling effect in the interface of heterogeneous nanobrush. To our relief, the magnetic heterogeneous nanobrush shows an excellent GMI ratio and high magnetic response at a low frequency.
Self-ordered anodic aluminum oxide (AAO) templates were prepared using the two-step anodization process in an oxalic acid solution (0.3 mol/L). The anodization potential was 40 V (20 V for sulfuric acid, 80 V for phosphoric acid). The process consisted of two distinct steps: in the first one, the high purity (99.9995%) aluminum foil was subjected to the first anodization for 40 min; after the selective removal of the alumina film formed on the surface of the Al anodized foil with an aqueous solution of 1.8% H2CrO4 and 6% H3PO4, the Al foil was subjected to the second anodization step for 6 h. Fe25Ni75 thin films were prepared by RF magnetron sputtering onto the surface of nanowire arrays with common base pressure below 3 × 10−5 Pa and processing Ar pressure of 0.4 Pa. The RF power was 140 W, and the time of deposition was 30 min. Moreover, the FeNi film would have to cover the top of AAO template, and the surface of the sample was conductive.
X-ray diffraction confirmed the composition of the nanowires array. Magneto-optic Kerr effect (MOKE) was used to obtain the surface magnetic properties of the composite structure. The surface topography and nanostructure were observed by scanning electron microscope (SEM). Micromagnetic simulations were performed with the three-dimensional object-oriented micromagnetic framework method. The exchange constants of the film and wires were 1.3 × 10−11 J/m and 1.75 × 10−11 J/m, respectively. The damping parameter α was 0.5, the mesh size was 5 × 5 × 5 nm3, and the saturation magnetization of permalloy film and Fe nanowires were 8.6 × 105 and 1.71 × 105 A/m, respectively. The ferromagnetic resonance was performed using an X-band spectrometer (JES-FA300; f = 9 GHz; JEOL Ltd., Tokyo, Japan). Before magnetoimpedance (MI) measurement, the samples were tailored into small pieces with length of 20 mm and width of 3 mm. An impedance analyzer (Agilent 4294A; Agilent Technologies Inc., CA, USA) was used in the four-terminal contact mode to measure the impedance (Z). All the electronic instruments were controlled using LabVIEW.
Results and discussion
It should be emphasized that not only the GMI ratio but also the magnetic response is important for high-performance sensor application. Figure 3b shows the magnetic response to the different compositions of nanowires. The sensitivity (S) of the GMI was defined as follows: S (%/Oe) = (ΔZ / Z) / ΔH, where ΔH is the change of the magnetic field. At very small external applied field, the field sensitivities of GMI effect of the nanobrush are 25%/Oe, 20%/Oe, 45%/Oe. Afterwards, it begins to decrease and display a value which is approximately equal to zero. The inset table shows the GMI ratios and sensitivities of several typical materials. The optimal structure and size is the FeNi film with 50-nm Co nanowire arrays which show a higher GMI ratio and more sensitive response than these amorphous wires, ribbon, and NiFe/Au/NiFe sandwich structure [27–31].
A new kind of exchange coupling effect is used to enhance the transverse moment distribution. A surprising GMI ratio and magnetic respond of heterogeneous nanobrush are found in the experiment. The diameter of the nanowires has obvious influence on the GMI characters of the nanobrush. The sample combined with 50 nm Co nanowires and Fe25Ni75 film shows the best GMI ratio and sensitivity, which could reach 270%/Oe and 45%/Oe, respectively. The phenomenon can be explained by the obvious distribution of transverse magnetic moments, which is induced by the exchange coupling effect between the interface of nanowires and film, and the exchange coupling effect can be regulated by the content of Co element of nanowire arrays. Micromagnetic stimulation shows the distribution of magnetic moments when the nanowire array act on the soft magnetic film. Out-of-plane FMR result confirms the different coupling effects of the different nanobrushes, which corresponds well with the GMI results of the nanobrushes.
JW and QL are professors of the Institute of Applied Magnetics, Key Laboratory for Magnetism and Magnetic Materials of the Ministry of Education, Lanzhou University. YZ and CM are Ph.D. students.
Sincere thanks goes to the National Basic Research Program of China (2012CB933101), National Science Fund of China (11074101, 51171075), the Fundamental Research Funds for the Central Universities (lzujbky-2012-k29 and lzujbky-2012-209), and the Program for New Century Excellent Talents in University.
- Phan MH, Peng HX: Giant magnetoimpedance materials: fundamentals and applications. Prog Mater Sci 2008, 53: 323–420. 10.1016/j.pmatsci.2007.05.003View Article
- Mohri K, Uchiyama T, Panina LV: Recent advances of micro magnetic sensors and sensing application. Sens Actuators A 1997, 59: 1–8. 10.1016/S0924-4247(97)80141-0View Article
- Atkinson D, Squire PT, Maylin MG, Gore J: An integrating magnetic sensor based on the giant magneto-impedance effect. Sens Actuators A 2000, 81: 82–85. 10.1016/S0924-4247(99)00091-6View Article
- Yabukami S, Mawatari H, Horikoshi N, Murayama Y, Ozawa T, Ishiyama K, Arai KI: A design of highly sensitive GMI sensor. J Magn Magn Mater 2005, 290: 1318–1321.View Article
- Tejedor M, Hernando B, Sanchez ML, Prida VM, Vazquez M: Magneto-impedance effect in amorphous ribbons for stress sensor application. Sens Actuators A 2000, 81: 98–101. 10.1016/S0924-4247(99)00095-3View Article
- Fernandez E, Kurlyandskaya GV, Garcia-Arribas A, Svalov AV: Nanostructured giant magneto-impedance multilayers deposited onto flexible substrates for low pressure sensing. Nanoscale Res Lett 2012, 7: 230–234. 10.1186/1556-276X-7-230View Article
- Uchiyama T, Mohri K, Itho H, Nakashima K, Ohuchi J, Sudo Y: Car traffic monitoring system using MI sensor built-in disk set on the road. IEEE Tran Magn 2000, 36: 3670–3672. 10.1109/20.908936View Article
- Honkura Y: Development of amorphous wire type MI sensors for automobile use. J Magn Magn Mater 2002, 249: 375–381. 10.1016/S0304-8853(02)00561-9View Article
- Kurlyandskaya GV, Sanchez ML, Hernando B, Prida VM, Gorria P, Tejedor M: Giant-magnetoimpedance-based sensitive element as a model for biosensors. Appl Phys Lett 2003, 82: 3053–3055. 10.1063/1.1571957View Article
- Usov NA, Antonov AS, Lagarkov AN: Theory of giant magneto-impedance effect in amorphous wires with different types of magnetic anisotropy. J Magn Magn Mater 1998, 185: 159–173. 10.1016/S0304-8853(97)01148-7View Article
- Morikawa T, Nishibe Y, Yamadera H, Nonomura Y, Takeuchi M, Taga Y: Giant magneto-impedance effect in layered thin films. IEEE Trans Magn 1997, 33: 4367–4372. 10.1109/20.620448View Article
- Kraus L: Theory of giant magneto-impedance in the planar conductor with uniaxial magnetic anisotropy. J Magn Magn Mater 1999, 195: 764–778. 10.1016/S0304-8853(99)00286-3View Article
- Brunetti L, Coisson M, Tiberto P, Vinai F, Chiriac H, Borza F: Comparison between magneto-impedance properties of Fe(73.5)Cu(3)Nb(1)Si(13.5)B(9) melt-spun and glass-covered wires. Sens Actuators A 2001, 91: 203–206. 10.1016/S0924-4247(01)00498-8View Article
- Zhukov A, Ipatov M, Zhukova V, Garcia C, Gonzalez J, Blanco JM: Development of ultra-thin glass-coated amorphous microwires for HF magnetic sensor applications. Phys Status Solidi A 2008, 205: 1367–1372. 10.1002/pssa.200778133View Article
- Sinnecker JP, Garcia JM, Asenjo A, Vazquez M, Garcia-Arribas A: Giant magnetoimpedance in CoP electrodeposited microtubes. J Mater Res 2000, 15: 751–755. 10.1557/JMR.2000.0108View Article
- Betancourt I, Valenzuela R, Vazquez M: Giant magnetoimpedance in Co-based microwires at low frequencies (100 Hz-13 MHz). J Appl Phys 2002, 91: 8423–8425. 10.1063/1.1447518View Article
- Chen G, Yang XL, Zeng L, Yang JX, Gong FF, Yang DP, Wang ZC: High-temperature giant magnetoimpedance in Fe-based nanocrystalline alloy. J Appl Phys 2000, 87: 5263–5265. 10.1063/1.373315View Article
- Zhukov A: Design of the magnetic properties of Fe-rich, glass-coated microwires for technical applications. Adv Funct Mater 2006, 16: 675–680. 10.1002/adfm.200500248View Article
- Park DG, Kim CG, Lee JH, Kim WW, Hong JH: Effect of ion irradiation on a Co-based amorphous ribbon. J Appl Phys 2007, 101: 09N109–09N109–3.
- Chen L, Zhou Y, Lei C, Zhou ZM, Ding W: Giant magnetoimpedance effect in sputtered single layered NiFe film and meander NiFe/Cu/NiFe film. J Magn Magn Mater 2010, 322: 2834–2839. 10.1016/j.jmmm.2010.04.038View Article
- Ren Y, Dai YY, Zhang B, Liu QF, Xue DS, Wang JB: Tunable magnetic properties of heterogeneous nanobrush: from nanowire to nanofilm. Nanoscale Res Lett 2010, 5: 853–858. 10.1007/s11671-010-9574-5View Article
- Debnath AK, Samanta S, Singh A, Aswal DK, Gupta SK, Yakhmi JV, Deshpande SK, Poswal AK, Suergers C: Growth of iron phthalocyanine nanoweb and nanobrush using molecular beam epitaxy. Physica E 2008, 41: 154–163. 10.1016/j.physe.2008.06.022View Article
- Schilp S, Ballav N, Zharnikov M: Fabrication of a full-coverage polymer nanobrush on an electron-beam-activated template. Angew Chem Int Ed 2008, 47: 6786–6789. 10.1002/anie.200801858View Article
- Ren Y, Liu QF, Li SL, Wang JB, Han XH: The effect of structure on magnetic properties of Co nanowire arrays. J Magn Magn Mater 2009, 321: 226–230. 10.1016/j.jmmm.2008.08.111View Article
- Zhan QF, Chen ZY, Xue DS, Li FS, Kunkel H, Zhou XZ, Roshko R, Williams G: Structure and magnetic properties of Fe-Co nanowires in self-assembled arrays. Phys Rev B 2002, 66: 134436–134441.View Article
- Panina LV, Mohri K, Uchiyama T, Noda M, Bushida K: Giant magneto-impedance in co-rich amorphous wires and films. IEEE Trans Magn 1995, 31: 1249–1260.View Article
- Knobel M, Sanchez ML, Gomez-Polo C, Marin P, Vazquez M, Hernando A: Giant magneto-impedance effect in nanostructured magnetic wires. J Appl Phys 1996, 79: 1646–1654. 10.1063/1.361009View Article
- Moron C, Garcia A: Giant magneto-impedance in nanocrystalline glass-covered microwires. J Magn Magn Mater 2005, 290: 1085–1088.View Article
- Viegas ADC, de Andrade AMH, Sommer RL, Jiang JS, Chien CL: Magneto-impedance in Fe73.5Cu1Nb3Si13.5B9 amorphous films at microwave frequencies. J Magn Magn Mater 2001, 226: 707–708.View Article
- Phan MH, Peng HX, Yu SC, Vazquez M: Optimized giant magnetoimpedance effect in amorphous and nanocrystalline materials. J Appl Phys 2006, 99: 08C505–08C505–3.
- De CD, Fry N, Orue I, Panina LV, Garcia-Arribas A, Barandiaran JM: Very large magnetoimpedance (MI) in FeNi/Au multilayer film systems. Sens Actuators A 2006, 129: 256–259. 10.1016/j.sna.2005.09.060View Article
- Tannous C, Gieraltowski J: Giant magneto-impedance and its applications. J Mater Sci: Mater Electro 2004, 15: 125–133.
- Chen DX, Munoz JL, Hernando A, Vazquez M: Magnetoimpedance of metallic ferromagnetic wires. Phys Rev B 1998, 57: 10699–10704. 10.1103/PhysRevB.57.10699View Article
- Diaz De Sihues M, Durante-Rincon CA, Fermin JR: A ferromagnetic resonance study of NiFe alloy thin films. J Magn Magn Mater 2007, 316: E46-E465.View Article
- Yalcin N, Aktas B, Ozdemir M, Durusoy HZ: An ESR study on amorphous NiFe films. Physica B 1997, 233: 251–258. 10.1016/S0921-4526(97)00297-4View Article
- Kurlyandskaya GV, Bhagat SM, Svalov AV, Fernandez E, Garcia-Arribas A, Barandiaran JM: Feni-based film nanostructures for high frequency applications: design and characterization. Solid State Phenom 2011, 168: 257–260.
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.